Ni(3)(Mo(2)O(8))(XO(3)) (X = Se, Te): the first nickel selenite- and tellurite-containing Mo4 clusters.
Jiang, Hai-Long; Xie, Zhi; Mao, Jiang-Gao; Inorganic chemistry 46 (2007) 6495–6501; doi:10.1021/ic700500q

data_4339268
_publ_section_title
;
 Ni(3)(Mo(2)O(8))(XO(3)) (X = Se, Te): the first nickel selenite- and
 tellurite-containing Mo4 clusters.
;
_journal_issue                   16
_journal_name_full               'Inorganic chemistry'
_journal_page_first              6495
_journal_page_last               6501
_journal_paper_doi               10.1021/ic700500q
_journal_volume                  46
_journal_year                    2007
_chemical_formula_sum            'Mo2 Ni3 O11 Te'
_chemical_formula_weight         671.61
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 103.228(7)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   9.562(3)
_cell_length_b                   8.756(3)
_cell_length_c                   10.082(3)
_cell_measurement_temperature    293(2)
_cell_volume                     821.7(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.988
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'Rigaku Mercury CCD'
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0226
_diffrn_reflns_av_sigmaI/netI    0.0235
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            3095
_diffrn_reflns_theta_full        27.46
_diffrn_reflns_theta_max         27.46
_diffrn_reflns_theta_min         2.08
_diffrn_standards_decay_%        <1.0%
_exptl_absorpt_coefficient_mu    13.254
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.5169
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    5.429
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       brick
_exptl_crystal_F_000             1232
_exptl_crystal_size_max          0.1400
_exptl_crystal_size_mid          0.1300
_exptl_crystal_size_min          0.0800
_refine_diff_density_max         1.224
_refine_diff_density_min         -0.696
_refine_diff_density_rms         0.186
_refine_ls_extinction_coef       0.00513(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.106
_refine_ls_matrix_type           full
_refine_ls_number_parameters     88
_refine_ls_number_reflns         1002
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.106
_refine_ls_R_factor_all          0.0186
_refine_ls_R_factor_gt           0.0175
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0219P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0413
_refine_ls_wR_factor_ref         0.0418
_reflns_number_gt                962
_reflns_number_total             1002
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic700500q-file002.cif
_cod_data_source_block           Ni-Mo-Te-O
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to
/usr/data/users/saulius/automatic-downloads/retrospective/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi-scan'
changed to 'multi-scan' according to
/usr/data/users/saulius/automatic-downloads/retrospective/ACS/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_cell_volume        821.7(4)
_cod_original_sg_symbol_H-M      C2/m
_cod_database_code               4339268